Journal of Saudi Chemical Society (2015) 19, 101–107
King Saud University
Journal of Saudi Chemical Society
Synthesis and characterization of polyaniline/
zeolite nanocomposite for the removal of
chromium(VI) from aqueous solution
* Corresponding author. Mobile: +964 7700278242.
E-mail address: email@example.com (O.A. Hasan).
Peer review under responsibility of King Saud University.
Production and hosting by Elsevier
1319-6103 ª 2012 Production and hosting by Elsevier B.V. on behalf of King Saud University. Open access under CC BY-NC-ND license.
Open access under CC BY-NC-N
Abdulsalam A. Shyaa a, Omar A. Hasan a,*, Ahmed M. Abbas b
a Polymer Research Unit, College of Science, Al-Mustansiriya University, Iraq
b Chemistry Department, College of Science, Misan University, Iraq
Received 27 November 2011; accepted 1 January 2012
Available online 9 January 2012
Abstract The synthesis, characterization and capacity studies of ion exchange resin capable of
coordinating with metal ion are reported. Zeolite was modified with conducting polyaniline by
the polymerization of anilinium cation in and out side of zeolite channels and a nanocomposite
of polyaniline/zeolite (PANI/zeolite) was obtained by the oxidative polymerization of anilinium cat-
ion with the zeolite structure. The product was characterized by UV–visible, FTIR, 1H NMR,
XRD, SEM and TGA techniques. From FTIR studies it was obtained that the composite has a high
content of PANI. SEM pictures in the present study show that the diameter of the PANI/zeolite
nanocomposite is between 300 and 600 nm.
Batch adsorption experiments were used to investigate the effect of various experimental param-
eters on the equilibrium adsorption of chromium(VI) on PANI/zeolite nanocomposite. The adsorp-
tion characteristics of the composite toward Cr(VI) in dilute aqueous solution were followed
spectrophotometrically. The effect of contact time, size of the sorbent and the concentration of
Cr(VI) in solution on the metal uptake behavior of the composite were studied. It has been observed
that the capacity of chromium adsorption on PANI/zeolite increases with initial metal concentra-
tion, the metal ion adsorption on surfactant is well represented by the Freundlich isotherm.
ª 2012 Production and hosting by Elsevier B.V. on behalf of King Saud University.
Environmental contamination by metals is a widespread prob-
lem, with sources of pollution arising from industrial activities.
Many toxic metal ions that are highly toxic for animals and
human beings have been discharged into the environment as
industrial wastes, causing serious soil and water pollution
(Lin and Junang, 2002). These metals are of significant impor-
tance as they are non-biodegradable and once released into the
environment, they can only be diluted or transformed, not de-
stroyed (Tramontina et al., 2001).
102 A.A. Shyaa et al.
Various methods have been proposed to remove heavy me-
tal ions from sea water and waste waters using ion-exchange
resin, adsorption (Fugiang and Baojiao, 2006; Li et al., 2005,
2009, 2010), electrolyte or liquid extraction, electrodialysis
(Qdais and Moussa, 2004), chemical precipitation (Karabulut
et al., 2002), membrane filtration (Saliba et al., 2000), Biosorp-
tion (Rao et al., 2002). Ion exchange/adsorption methods do
offer the most direct method for producing the highest quality
treated water (Ko et al., 2000).
Zeolite is a crystalline aluminosilicate with 3-dimensional,
open anion framework consisting of oxygen sharing TO4,
Tetrahedral, where T is Si or Al. Their framework structure
contains interconnected voids that are filled with cations usu-
ally from group IA or IIA which can be exchanged with other
cations (such as anilinium cations) (Olad et al., 2010; Ramos et
al., 2008). Due to their unique physical and chemical properties
(crystallinity, thermal stability, well-defined cage structure of
molecular size, ion exchange, etc.) zeolites have been used as
heavy metal adsorbents, as chemical sieves and as water
softeners (Zeng et al., 2010; Hong, 2009; Sulimenko et al.,
The main objectives of this study are to develop inexpensive
and effective metal ion adsorbents, also to explore the
feasibility of using zeolite nanocomposite for the removal of
toxic heavy metals from waste waters.
Fourier Transform Infrared Spectrometer (FTIR) was used for
the determination of functional groups in PANI/zeolite using
KBr pellets. The pellets were analyzed with FTIR Spectrome-
ter (Shimadzu 8400S) in transmittance (%) mode in the range
UV–visible spectra were taken on T80 double beam spectro-
photometer. The morphology of the prepared materials was
examined on Inspect� S50-scaning electron microscope
(SEM). Thermogravimetric analysis (TGA) was performed
using Shimadzu TGA 60, measurements were carried out in
N2 atmosphere under 50 ml/min flow rate and a heating rate
of 20 �C/min from room temperature to 800 �C. X-ray diffrac-
tion pattern was measured on XRD 7000 Shimadzu X-ray
Aniline, ammonium persulfate were purchased from Merck.
Aniline was distilled under reduced pressure and stored at
5 �C. Zeolite was obtained from Aldrich.
2.3. Synthesis of polyaniline/zeolite nanocomposite
PANI/zeolite nanocomposites were synthesized via an in situ
oxidative polymerization (Marjanovic et al., 2009), in which
the natural zeolite was ground and sieved with 100 lm of
sieve. Then 1.5 g of zeolite was vigorously stirred in
200 mL of 1 M HCl for 24 h. Ten grams (107.5 mmol) of
aniline was dispersed in matures of HCl and zeolite with
continuous stirring for 24 h. Ammonium persulphate
(67 mmol) was dissolved in 1 M HCl (200 ml) and dropped
into the Beaker. The mixture was kept at constant stirring
and the solution is placed inside an ice bath maintaining stir-
ring for another 24 h. When the reaction was completed, the
dark green precipitate resulting from the polymerization
reaction was filtered and washed with distilled water, acetone
and methanol sequentially in order to remove the excess of
initiator, monomer, and oligomer. The precipitate was then
dried overnight in vacuum oven at 60 �C.
2.4. Adsorption experiments
The Cr(VI) solutions were prepared in different concentrations
that ranged from 20 to 100 ppm by diluting K2CrO4 stock
solution (1000 ppm) appropriately as necessary.
To determine the conditions that achieve the maximum
amount of metal ion removal, adsorption experiments were
done. Reaction isotherm and kinetics were also conducted in
Various amounts of PANI/zeolite powder were introduced
into a 100 ml volumetric flasks and 50 ml Cr(VI) solution of
different concentrations were added. The adsorption tests were
conducted in thermostated water bath shaker at a fixed tem-
perature of 30 �C.
The efficiency of Cr(VI) removal was calculated as
Removal efficiency ¼ 100Ci � Cf
where Ci and Cf are the initial and final concentrations in ppm,
If q is the amount of metal adsorbed per specific amount of
adsorbent (mg/g). The sorption capacity of time t, qt (mg/g)
was obtained as follows:
vðCi � CfÞ
where Ci and Cf (ppm) were the liquid phase concentrations of
solutes at initial and given time t, v was the solution volume
and m is the mass of PANI/zeolite (g).
3. Results and discussion
3.1. Characterization of PANI/zeolite nanocomposite
Zeolite was modified through the polymerization of aniline
monomer inside and outside of zeolite channel, where the
exchangeable cations were replaced by anilinium ions. The
polymerization of aniline is achieved only in an acidic medium
in the presence of hydrochloric acid where aniline exists as ani-
linium cations. Peroxy disulfate was used as an oxidant for the
anilinium ion due to the higher solubility in water of its ammo-
nium salt. To minimize the presence of residual aniline and to
obtain the best yield of PANI, 1.25 peroxydisulfate/aniline ra-
tio is recommended (Fu and Elsenbaumer, 1994), the oxidation
of aniline is exothermic so the temperature of the reaction mix-
ture can be used to monitor the progress of the reaction (Hong,
2009; Sulimenko et al., 2001). In this study, polyaniline was